General

Property | Value | Condition |
---|---|---|

Density | 2.69 g/cm³ Show Material materials with Density of 2.69 g/cm³ | H34 |

2.7 g/cm³ Show Material materials with Density of 2.7 g/cm³ | H34 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Comment |
---|---|---|---|---|---|

Compressive modulus | 71.0 MPa Show Material materials with Compressive modulus of 71.0 MPa | H34 | |||

Elastic modulus | 70 GPa Show Material materials with Elastic modulus of 70 GPa | H34 | |||

71.0 GPa Show Material materials with Elastic modulus of 71.0 GPa | H34 | ||||

Elongation | -195 °C | 30 % Show Material materials with Elongation of 30 % | H34 | Elongation in 50 mm | |

-80 °C | 21 % Show Material materials with Elongation of 21 % | H34 | Elongation in 50 mm | ||

4.0 % Show Material materials with Elongation of 4.0 % | H34 | AA Standards, ASTM B209 | A50 | ||

4.0 % Show Material materials with Elongation of 4.0 % | H34 | AA Standards, ASTM B234 | A100 | ||

5.0 % Show Material materials with Elongation of 5.0 % | H34 | AA Standards, ASTM B209 | A50 | ||

6.0 % Show Material materials with Elongation of 6.0 % | H34 | AA Standards, ASTM B209, ASTM B547 | A50 | ||

6.0 % Show Material materials with Elongation of 6.0 % | H34 | AA Standards, ASTM B234 | A100 | ||

7.3 % Show Material materials with Elongation of 7.3 % | H34 | ||||

9.0 % Show Material materials with Elongation of 9.0 % | H34 | AA Standards, ASTM B209 | A100 | ||

10.0 % Show Material materials with Elongation of 10.0 % | H34 | AA Standards, ASTM B209, ASTM B547 | A50 | ||

0 °C | 18 % Show Material materials with Elongation of 18 % | H34 | Elongation in 50 mm | ||

24 °C | 16 % Show Material materials with Elongation of 16 % | H34 | Elongation in 50 mm | ||

100 °C | 18 % Show Material materials with Elongation of 18 % | H34 | Elongation in 50 mm | ||

150 °C | 32 % Show Material materials with Elongation of 32 % | H34 | Elongation in 50 mm | ||

205 °C | 45 % Show Material materials with Elongation of 45 % | H34 | Elongation in 50 mm | ||

260 °C | 80 % Show Material materials with Elongation of 80 % | H34 | Elongation in 50 mm | ||

315 °C | 110 % Show Material materials with Elongation of 110 % | H34 | Elongation in 50 mm | ||

370 °C | 130 % Show Material materials with Elongation of 130 % | H34 | Elongation in 50 mm | ||

Hardness, Brinell | 81.0 [-] Show Material materials with Hardness, Brinell of 81.0 [-] | H34 | AA Standards | ||

81.0 [-] Show Material materials with Hardness, Brinell of 81.0 [-] | H34 | 500 kg load, 10 mm ball | |||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 5000 Series Aluminium | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 5000 Series Aluminium | |||

Shear modulus | 26.0 - 26.5 GPa Show Material materials with Shear modulus of 26.0 - 26.5 GPa | Typical for Wrought 5000 Series Aluminium | |||

Shear strength | 179.0 MPa Show Material materials with Shear strength of 179.0 MPa | H34 | |||

Tensile strength | -195 °C | 435 MPa Show Material materials with Tensile strength of 435 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

-80 °C | 317 MPa Show Material materials with Tensile strength of 317 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

270.0 - 325.0 MPa Show Material materials with Tensile strength of 270.0 - 325.0 MPa | H34 | AA Standards, ASTM B209, ASTM B547 | |||

270.0 MPa Show Material materials with Tensile strength of 270.0 MPa | H34 | AA Standards, ASTM B234 | |||

300.0 MPa Show Material materials with Tensile strength of 300.0 MPa | H34 | ||||

0 °C | 303 MPa Show Material materials with Tensile strength of 303 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

305.0 MPa Show Material materials with Tensile strength of 305.0 MPa | H34 | AA Standards | |||

24 °C | 303 MPa Show Material materials with Tensile strength of 303 MPa | H34 | |||

100 °C | 295 MPa Show Material materials with Tensile strength of 295 MPa | H34 | |||

150 °C | 235 MPa Show Material materials with Tensile strength of 235 MPa | H34 | |||

205 °C | 180 MPa Show Material materials with Tensile strength of 180 MPa | H34 | |||

260 °C | 117 MPa Show Material materials with Tensile strength of 117 MPa | H34 | |||

315 °C | 74 MPa Show Material materials with Tensile strength of 74 MPa | H34 | |||

370 °C | 40 MPa Show Material materials with Tensile strength of 40 MPa | H34 | |||

Unlock all property charts | |||||

Yield strength | -196 °C | 285 MPa Show Material materials with Yield strength of 285 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |

-80 °C | 250 MPa Show Material materials with Yield strength of 250 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

-28 °C | 240 MPa Show Material materials with Yield strength of 240 MPa | H34 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

200.0 MPa Show Material materials with Yield strength of 200.0 MPa | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 | RP02 | ||

240.0 MPa Show Material materials with Yield strength of 240.0 MPa | H34 | AA Standards | RP02 | ||

240.0 MPa Show Material materials with Yield strength of 240.0 MPa | H34 | ||||

24 °C | 240 MPa Show Material materials with Yield strength of 240 MPa | H34 | |||

100 °C | 235 MPa Show Material materials with Yield strength of 235 MPa | H34 | |||

149 °C | 195 MPa Show Material materials with Yield strength of 195 MPa | H34 | |||

204 °C | 130 MPa Show Material materials with Yield strength of 130 MPa | H34 | |||

260 °C | 75 MPa Show Material materials with Yield strength of 75 MPa | H34 | |||

316 °C | 50 MPa Show Material materials with Yield strength of 50 MPa | H34 | |||

371 °C | 29 MPa Show Material materials with Yield strength of 29 MPa | H34 | |||

Unlock all property charts |

Thermal

Property | Value | Condition | Comment |
---|---|---|---|

Coefficient of thermal expansion | 2.4e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.4e-05 1/K | H34 | |

Max service temperature | 150.0 °C Show Material materials with Max service temperature of 150.0 °C | Typical for Wrought 5000 Series Aluminium | |

Melting point | 600.0 °C Show Material materials with Melting point of 600.0 °C | H34 | |

Specific heat capacity | 900.0 J/(kg·K) Show Material materials with Specific heat capacity of 900.0 J/(kg·K) | H34 | |

Thermal conductivity | 130.0 W/(m·K) Show Material materials with Thermal conductivity of 130.0 W/(m·K) | H34 |

Electrical

Property | Value | Comment |
---|---|---|

Electrical conductivity | 18000000.0 - 31000000.0 S/m Show Material materials with Electrical conductivity of 18000000.0 - 31000000.0 S/m | Typical for Wrought 5000 Series Aluminium |

Electrical resistivity | 3.3e-08 - 5e-08 Ω·m Show Material materials with Electrical resistivity of 3.3e-08 - 5e-08 Ω·m | Typical for Wrought 5000 Series Aluminium |

Chemical properties

Property | Value | Condition | Related Standards |
---|---|---|---|

Aluminium | 94.5 - 97.1 % Show Material materials with Aluminium of 94.5 - 97.1 % | H34 | |

Chromium | 0.05 - 0.2 % Show Material materials with Chromium of 0.05 - 0.2 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Copper | 0.1 % Show Material materials with Copper of 0.1 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Iron | 0.40 % Show Material materials with Iron of 0.40 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

0.4 % Show Material materials with Iron of 0.4 % | H34 | ||

Magnesium | 2.4 - 3.0 % Show Material materials with Magnesium of 2.4 - 3.0 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Manganese | 0.5 - 1.0 % Show Material materials with Manganese of 0.5 - 1.0 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Other | 0.15 % Show Material materials with Other of 0.15 % | H34 | |

Silicon | 0.25 % Show Material materials with Silicon of 0.25 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Titanium | 0.2 % Show Material materials with Titanium of 0.2 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Zinc | 0.25 % Show Material materials with Zinc of 0.25 % | H34 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Technological properties

Property | ||
---|---|---|

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: no damage during operation and laboratory tests, general: very good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (O, H32, H111), sufficient (H34) | |

Workability | general (condition): good (O), acceptable (H32, H34, H111) |